Se ha denunciado esta presentación.
International Journal of JOURNAL OF MECHANICAL ENGINEERING AND INTERNATIONAL Mechanical Engineering and Technology (IJMET), ISSN 0976 – 6340(Print), ISSN 0976 – 6359(Online) Volume 3, Issue(IJMET) (2012) © IAEME TECHNOLOGY 3, Sep- DecISSN 0976 – 6340 (Print)ISSN 0976 – 6359 (Online) IJMETVolume 3, Issue 3, Septmebr - December (2012), pp. 01-06© IAEME: www.iaeme.com/ijmet.htmlJournal Impact Factor (2012): 3.8071 (Calculated by GISI) ©IAEMEwww.jifactor.com TRIBOLOGICAL TESTING REGIME FOR ESTABLISHING EFFICIENCY OF ZDDP IN PRESENCE OF WEAR DEBRIS UNDER LUBRICATED SLIDING METALLIC CONTACTS-A REVIEW Intezar Mahdi1,#, Rajnish Garg2 and Anupam Srivastav1 1 Department of Mechanical Engineering, SET, IFTM University, Moradabad, India 2 University of Petroleum & Energy Studies, Dehradun, India # Corresponding Author/Email: firstname.lastname@example.org ABSTRACT ZDDP has established itself over last sixty years as most prominent anti wear additive, in addition to being anti-oxidant and anti-corrosion agent in automotive lubricants. This paper presents a critical review of state of the art in the qualitative and quantitative effectiveness of Zinc Dialkyl Dithio Phosphate (ZDDP) as anti-wear additive when in contact with wear debris under lubricated metallic sliding condition. The result of this study gives a condition monitoring parameter to evaluate the health and condition of lubricants and thus that of tribo- surfaces. Key words: Lubrication, Wear Debris, ZDDP, 1. INTRODUCTION Liquid lubricants are low-viscosity, low shear strength natural or artificial substances introduced between two moving surfaces to reduce the friction between them as well as reducing wear, thereby improving efficiency and service life. They additionally may also dissolve or transport foreign particles and distribute heat. Internal combustion engines of motor vehicles and similar such powered equipment are the single largest user of such lubricants, in the form of motor oil. Lubricants generally contain 90% base oil (most often petroleum fractions, called mineral oils) and less than 10% additives. Vegetable oils or synthetic liquids such as hydrogenated polyolefins, esters, silicone, fluorocarbons and many others are sometimes used as base oils. In view of arrival of efficient engines with advanced designs, such as overhead valves and V 6 or V 8 engines with increased compression ratio, lubricating oils with no or ordinary additives were rendered useless because the stresses on engine components such as the cam mechanisms commonly working at 1m/s speed increased to as high as 1 GPa . Also, the 1
International Journal of Mechanical Engineering and Technology (IJMET), ISSN 0976 –6340(Print), ISSN 0976 – 6359(Online) Volume 3, Issue 3, Sep- Dec (2012) © IAEMEdemand for light weight and high speed automobiles resulted in shift to material selection forengine components from Steels to Aluminum alloys, again increasing demand for betterlubricants in view of poor wear resistance of Al alloys. Similarly, poorer load bearingcapability of Babbit, when used in high horse power engines resulted in use ofcadmium/silver, cadmium/nickel and copper/lead as stronger bearing material but withinferior wear and corrosion resistance. These factors led to discovery and usage of ZincDialkyl Dithio Phosphate (ZDDP) as an anti-wear additive for motor vehicle lubricants asearly as 1941. ZDDP is used as a bearing passivatorto coat a metal in order to reduce thechemical reactivity of its surface. ZDDP concentration in such cases is low-less than 0.3%. Italso has anti-oxidant when added in oils. Moreover, it is also effective anti-wear agent, an EPadditive for heavily loaded steel-on-steel sliding mechanisms such as camshafts and valvelifters or tappets . It reduces the risk of metal-to-metal contact, which can lead to increasedheat, result in oxidation and negatively affect the film strength.In order to improve the understanding as to how wear and friction are affected bysimultaneous interaction of variables such as loading, oil contamination due to wear debris,ZDDP presence in oil and the tribological system configuration, it is imperative to review thework, which has been carried out for each of these factors. Such understanding should help insetting up dedicated experiments to understand the synergic effect of these factors. Also, itshould elucidate in establishing a clear condition monitoring parameter for such tribo-systems. 2. LUBRICANT ADDITIVES AND WEAR DEBRISIt is of paramount importance to understand that using more oil additives is not always better.Sometimes when more additive is added into the oil, there is not much benefit gained, and tothe contrary, the performance actually deteriorates. Moreover, in some cases, increasing thepercentage of a particular additive may improve one property of lubricating oil and degradeanother property. In addition, if the concentrations of additives in lubrication oils becomemore than desired and unbalanced, overall oil quality may also get affected. Mostimportantly, some additives may compete with each other in the same volume of oil thusaffecting their surface chemistry. It is seen in cases such as when higher concentration of ananti-wear additive is blended with the lubrication oil, it may suppress a corrosion inhibitorpresent in the oil, resulting in an increase in corrosion-related problems .In the past two decades, the role of lubricant additives in wear reduction has been extensivelyinvestigated in various research studies all across the world. These studies have differentstudy parameters and have established different facts about effectiveness of different types ofadditives in different conditions. Due to such a vast area of application, no study couldclearly identify or zero in to a very limited range of additives which can be recommended formost applications and conditions. It has been established through such studies that wearreduction is achieved in particular conditions when lubricant additives are added in oils. Butstudies have also shown that additives (ZDDP) reduces wear in lubricated sliding only underlow loads and when loads are high, wear increases at high loads indicating change in surfacedue to chemical action of additive in oil [ 5-6].Presence of contaminant is another significant factor to be considered in lubricated systems,particularly when they are hard and abrasive. Presence of any such contaminants in thelubricating oils or greases are found to be one of the major causes of tribo-elements failure 2
International Journal of Mechanical Engineering and Technology (IJMET), ISSN 0976 –6340(Print), ISSN 0976 – 6359(Online) Volume 3, Issue 3, Sep- Dec (2012) © IAEME, Investigation into such test conditions have proved that such contaminants increase wearof the sliding contacting surfaces and also the friction coefficient. It is also found that thenature of contacting materials determine the severity of such behavior [8-9]. Solidcontaminants are generally grouped into three categories. The external contaminants, whichenter the lubricating oils through air, fuel and fresh oil, are put in first categories. The secondcategory of contaminants is that which are generated due to friction and wear of the rubbingsurfaces, which are generally known as wear debris and which this work is focusing on. Thecontaminants, which get introduced into the tribo-system initially during manufacturing andassembly of such tribo-systems, are the third category of contaminants .Considering wear debris, which as stated above, circulates during operation of machine,getting flushed into the system and if the operating contact pressures are high and oil filmsare small, then damage even the hardest gear, bearing or cam surfaces. This damage can leadto contact fatigue or wear, and thus premature failure of the whole machine. Further, onefailure can result in the generation of further wear debris, often in very great quantities, thatthen can have effect on other parts of the tribological system.These wear debris particles vary from sub-micron to millimeter in size whereas the shapestend to be blocky and angular. Generally, the nature of circulating lubricant system is suchthat only the particles less than around 100µm find their way into machine components(larger particles settle quicker in a lubrication sump). However, in case of grease lubricatedbearings, such as on a mining conveyor belt may see much larger particles. Figure 1 givesconditions under which some prominent tribo-elements will give rise to a particular nature ofwear debris under specific tribological condition.Table 1: Example of Type of Component and Nature of Wear Debris Example of Tribo- Nature of Wear Debris Type of Component Element Loaded, moving components in Ferrous particles of Rolling bearings, gear which load is concentrated in a various size and shapes teeth, cams and tappets non-confirmed contact Ferrous flakes less than Loaded, moving components in Piston rings and 150 µm across, and fine which load is concentrated in a cylinders splines, gear iron or iron oxide small area couplings particles Usually very small and ferrous and non-ferrous Loaded, moving components Plain bearings, pistons flakes and particles, with the load spread over a and cylinders bearing fatigue can give large area rise to larger flakes 3
International Journal of Mechanical Engineering and Technology (IJMET), ISSN 0976 –6340(Print), ISSN 0976 – 6359(Online) Volume 3, Issue 3, Sep- Dec (2012) © IAEME3. ZINC DIALKYL DITHIO PHOSPHATES (ZDDPS) AND THEIR EFFECT ON WEAR DEBRISZinc Dialkyl Dithio Phosphates (ZDDPs are, till now, the most important and widely usedanti-wear and anti-oxidant additive, which is added to engine oils. Generally, ZDDP is amixture of neutral ZDDP and basic ZDDP. Figure 1 shows the structure of the neutral ZDDP(monomer) having chemical formula [(RO)2PS2]2Zn. Also, the neutral ZDDP can exist as adimer, or an infinite linear polymer in the solid state depending upon nature of the alkylgroup.Figure 1: Structure of Neutral ZDDPIt is known from the literature, that ZDDP acts as an anti-wear additive in lubricants in threemain ways (i) by forming a mechanically protective film; (ii) by removing corrosiveperoxides or peroxy-radicals; (iii) by ‘‘digesting’’ hard and thus abrasive iron oxide. Rubbing surfaces of engines are protected against wear by anti-wear ZDDPs’films, generatedin situ, which act as sacrificial films when being rubbed. These films are dynamic as they areconstantly regenerated in a rubbing environment [13-14]. It has been found that the productsproduced as a result breakdown of ZDDPs during sliding, (not the ZDDPs itself) provides theantiwear protection to sliding steel surfaces. ZDDPs form tribo-films by two mechanisms,one when it decomposes upon rubbing as well as second due to thermal decomposition.These films have an amorphous polyphosphate glass structure .Studies on such anti-wear films generated from neutral and basic ZDDP salts do have anysubstantial difference. The wear scar diameter and the P and S chemical environment in thetribo film has been found to be similar, however, the chemical composition has differences.Basic ZDDP mostly produce wear debris either of un reacted ZDDP or of a linkage isomer ofZDDP (LI-ZDDP), and zinc polyphosphate. On the other hand, the wear debris of neutralZDDP is exclusively composed of zinc polyphosphate (and sulphur species) . Also, moreiron is reported in the wear debris with basic ZDDP, a possible indication of the iron contentof the tribo film. Differences in chemical structure are also reported in case of thermal films.Neutral ZDDP forms polyphosphates at 150oC, whereas basic ZDDP forms the same productat higher temperature of 175oC.Anti-wear chemistry of ZDDPs has also been studied by different workers. The zincpolyphosphate glass, formed as breakdown product, is attributed to digestion of abrasiveparticles during sliding. The driving force for this tribo-chemical reaction is not temperaturebut entropy due to mechanical mixing at the atomic scale . In another substantial work, itis reported that the reaction products of ZDDP, which are phosphates, are present as shortchain phosphates, which is a mix of iron and zinc phosphates. It has greater proportion ofphosphates compared to sulfur species . In one of the most important and recent study tocompare the anti-wear properties of ZDDP and fluorinated ZDDP, it is established that thewear debris produced in presence of both types of additives, is essentially amorphous but 4
International Journal of Mechanical Engineering and Technology (IJMET), ISSN 0976 –6340(Print), ISSN 0976 – 6359(Online) Volume 3, Issue 3, Sep- Dec (2012) © IAEMEcontains nano crystalline particles of Fe3O4Also, F-ZDDP results in lower wear incomparison to ZDDP under identical tribological conditions .4. FUTURE RESEARCH STRATEGY FOR CONTAMINATED TRIBOLOGICAL ENVIRONMENTSIn spite of substantial research efforts, complete tribo-mechanism of ZDDP and its reactionmechanism by which anti-wear tribo-films are formed on the tribo-surfaces is not totallyunderstood. Problems associated with lack of understanding gets magnified due to the factthat ZDDP goes through complex reactions which are dependent on many variables and anti-wear process being multidisciplinary, involving metallurgy, chemistry, metrology andmechanical areas. It is therefore important to properly set up testing regimes, wherein wearparticles of all nature, size and geometries are artificially introduces into the testing system,stating with base oils and going up to oils contacting different types and concentrate ofadditives.Such a comprehensive testing environment will clearly identify the metallurgicalcharacteristics of these tribo-surfaces when wear debris of different sizes, quantities andproperties are present in lubricating oils, which contain ZDDP as anti-wear additive indifferent concentrations, alongside other additives as well. It shall also help in establishingthe extent of tribological effectiveness in presence of wear debris, which is an integral part ofany lubricating oil, striving to have longer service life. The information assimilated throughsuch comprehensive tests will explain synergy between ZDDP and other additives and alsoserve as a good condition monitoring tool. The authors have been working on suchexperiments, which shall soon be completed and the results will increase our understandingof such complex problems.5. REFERENCES1. H.Spedding and R.C Watkins, “The anti wear mechanism of ZDDP’s Part I,Tribology International, Vol. 15, 1, pp. 9-12. 1982.2. Dave Sutton, “ZDDP: When, Where, What, Why, How?”http://www.enginebuildermag.com/Article/98566, 26.03.12.3. P. Oviedo, “The Critical Role of Additives in Lubrication” Machinery Lubrication,http://www.machinerylubrication.com/Read/28980/additives-lubrication-role, 8-11-2012.4. F. Wang, Y. Cheng and D. Guan, “On the Tribological Behavior and Surface Analysisof a Sliding PSZ Ceramic-Steel Pair”, Journal of Tribology, Transactions of the ASME, 117,pp. 548-552, 1995.5. S. Jahanmir, “Wear Reduction and Surface Layer Formation by a Zddp Additive”,Journal of Tribology, Transactions of the ASME, 109, pp. 577-586, 19876. M. M. Maru and D. K. Tanaka, “Influence of Loading, Contamination and Additiveon the Wear of a Metallic Pair under Rotating and Reciprocating Lubricated Sliding” J. of theBraz. Soc. of Mech. Sci. & Eng., Vol. XXVIII, No. 3, pp. 278-285, July-September 2006,7. W. Ali, and M. Mousa, “Experimental Study of Wear and Friction Caused ByAbrasive Contaminants and Fuel Dilution in Lubricating Oil”, 5th International Congress OnTribology EUROTRIB 89, Helsinki, Finland, pp. 437-431, June 13, 1988.8. R.L Mehan, “The Wear of Selected Materials in Mineral Oil Containing a SolidContaminant”, Wear, 124, pp. 65-85, 1988. 5
International Journal of Mechanical Engineering and Technology (IJMET), ISSN 0976 –6340(Print), ISSN 0976 – 6359(Online) Volume 3, Issue 3, Sep- Dec (2012) © IAEME9. R.L Mehan, P.L Flynn and A.W Glammarise, , “Evaluation of Piston Ring Materialsin Oil Containing an Abrasive using a Ring-On-Block Test Machine”, Wear, 147, pp. 41-57,199110. A. M. Sheikh, M. I. Khashaba and W. Y. Ali, “Reducing the Mechanical Wear in aDusty Environment (Cement Factory)”, International Journal of Engineering & Technology(IJET-IJENS),Vol: 11 No: 06, pp. 166-172, December 2011.11. M. Kastelan-Macan, M. Petrovic, I. Haiduc, "Stereochemical Aspects of Phosphor-1,1-Dithiolato Metal Complexes (Dithiophosphates, Dithiophosphinates): CoordinationPatterns, Molecular Structures and Supramolecular Associations," Polyhedron, 14, p. 3389-3389-3472.199512. R. Mourhatch, “Triboilogical and Anti-wear Mechanisms of Fluorinated zincDialkylDithiophosphate in Comparison to ZDDP in Engine Oils”, PhD Thesis, TheUniversity of Texas at Arlington, USA, May 200813. W.J. Bartz, “Engine Oils and Automotive Lubrication”, Marcel Dekker Inc.,NewYork, 1993).14. D. Klamann ed., Lubricants and related Products: Synthesis, Properties, Applications,International Standards, VerlagChemie, Deerfield Beach, FL, 1984.15. G. Pereiraa, A. Lachenwitzera, M.A. Nichollsa, M. Kasraia, P.R. Nortona, and G. DeStasiob, “Chemical characterization and nanomechanical properties of anti-wear filmsfabricated from ZDDP on a near hypereutectic Al–Si alloy”, Tribology Letters, Vol. 18, No.4, pp. 411-427, April 2005.16. K. Varlot, M. Kasrai, J.M. Martin, B. Vacher, G.M. Bancroft E.S. Yamaguchi andP.R. Ryason, “Antiwear film formation of neutral and basic ZDDP: influence of the reactiontemperature and of the concentration”, Tribology Letters, Volume 8, No 1, pp. 9-16(8), 200017. Jean Michel Martin , Tasuku Onodera , ClotildeMinfray, FabriceDassenoyand AkiraMiyamoto, “ The origin of anti-wear chemistry of ZDDP”, Faraday Discussions., 156, pp.311-323, 201218. B. H. Kim, R. Mourhatch, P. B. Aswath, “Properties of Tribofilms Formed WithAshlessDithiophosphate and Zinc DialkylDithiophosphateUnder Extreme PressureConditions”. Vol. 268, Issues 3–4, , pp. 579–591, February 2010.19. R.Mourhatch, and P. B. Aswath, “Tribological behavior and nature of tribofilmsgenerated from fluorinated ZDDP in comparison to ZDDP under extreme pressureconditions—Part 1: Structure and chemistry of tribofilms”, Tribology International, Volume44, Issue 3, , p. 187–200 March 2011 6